Research Article Microstructure, Mechanical, and Research Article Microstructure, Mechanical, and...
Embed Size (px)
Transcript of Research Article Microstructure, Mechanical, and Research Article Microstructure, Mechanical, and...
Research Article Microstructure, Mechanical, and Biological Properties of Porous Poly(vinylidene fluoride) Scaffolds Fabricated by Selective Laser Sintering
Wei Huang,1,2 Pei Feng,2 Chengde Gao,2 Xiong Shuai,3 Tao Xiao,4,5
Cijun Shuai,2,4 and Shuping Peng1,6
1Hunan Provincial Tumor Hospital and the Affiliated Tumor Hospital of Xiangya School of Medicine, Central South University, Changsha 410013, China 2State Key Laboratory of High Performance Complex Manufacturing, Central South University, Changsha 410083, China 3State Key Laboratory of Powder Metallurgy, Central South University, Changsha 410083, China 4Orthopedic Biomedical Materials Institute, Central South University, Changsha 410083, China 5Department of Orthopedics, The Second Xiangya Hospital, Central South University, Changsha 410011, China 6School of Basic Medical Science, Central South University, Changsha 410078, China
Correspondence should be addressed to Cijun Shuai; firstname.lastname@example.org and Shuping Peng; email@example.com
Received 26 January 2015; Revised 23 April 2015; Accepted 27 April 2015
Academic Editor: Piotr Wilczek
Copyright © 2015 Wei Huang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Porous poly(vinylidene fluoride) (PVDF) scaffolds were prepared by selective laser sintering. The effects of laser energy density, ranging from 0.66 to 2.16 J/mm2, on microstructure and mechanical properties were investigated. At low energy density levels, PVDF particles could fuse well and the structure becomes dense with the increase of the energy density. Smoke and defects (such as holes) were observed when the energy density increased above 1.56 J/mm2 which indicated decomposition of the PVDF powder. The scaffolds appeared to be light yellow and there was a reduction in tensile strength. The fabricated scaffolds were immersed into simulated body fluid for different time to evaluate biostability. In addition, MG63 cells were seeded and cultured for different days on the scaffolds. The testing results showed that the cells grew and spread well, indicating that PVDF scaffolds had good biocompatibility.
Autografts were the gold standard for bone transplantation, but their existing problems, for example, finite availabil- ity and donor site complication, had limited their clinical application [1–3]. Hence artificial bone had been used for bone regeneration. Tridimensional porous scaffolds played a crux role in synthetic bone, because the scaffolds could imitate the bone constructions and role of the extracellular matrix and endorse cell conglutination, multiplication, and differentiation. Besides they could transport nutrient and metabolic waste [4–7].
Scaffolds were fabricated by some conventional methods which mainly contained solvent casting, injection molding,
and electrospinning [8, 9]. However, these methods required a separate mold for exterior geometry and could not control over the porous architecture precisely . Solid freeform fabrication (SFF) methods could precisely control over the objects external shape and internal pore interconnectivity [11–16]. Selective laser sintering (SLS), as a family member of the SFF methods, employed a laser to selectively sinter thin layers of powder materials to form solid 3D objects [17, 18].
Poly(vinylidene fluoride) (PVDF) was a biocompatibility polymer. Zhang et al.  proved that PVDFpossessed hemo- compatibility and prepared PVDF hollow fiber hemodial- ysis membranes. Agyemang et al.  had found that PVDF-calcium phosphate composite scaffolds had potential applications in tissue engineering. Guo et al.  used
Hindawi Publishing Corporation International Journal of Polymer Science Volume 2015, Article ID 132965, 9 pages http://dx.doi.org/10.1155/2015/132965
2 International Journal of Polymer Science
Table 1: The SLS process parameters.
Parameters Value Spot diameter (mm) 0.8 Scan space (mm) 3.0 Layer thickness (mm) 0.1∼0.2
polyurethane/polyvinylidene fluoride scaffolds for trauma recovery applications.
In this study, PVDF scaffolds were fabricated via SLS for bone regeneration, and the effects of the laser energy density on microstructure and mechanical performance were stud- ied with scanning electron microscopy (SEM), a universal testing system, respectively. The biostability was evaluated by immersing the scaffolds into SBF. Besides, MG63 cells were planted on PVDF scaffolds and in vitro cell action, containing cell attachment and multiplication, was researched.
2. Materials and Methods
2.1. Material. PVDF powder (𝑀 𝑤 = 275,000 g/mol) was
purchased from Huangjiang Huayi Plastics Material Co., Guang Dong, China. Density was 1.75–1.78 g/cm3. It had a melting point of 170∘C and the long-term use temperature of −40∼150∘C, and the crystallinity index was approximately 50%.
2.2. Fabrication. Scaffolds were fabricated using a home- made SLS system which has been reported previously [22, 23]. When a process was developed for fabricating synthetic bone scaffolds, process parameters should be suitable. An important factor to the success of the sintering process was the laser energy density (ED). It was defined by
ED = 𝑃 𝑉 × 𝐷
(J/mm2) , (1)
where the laser energy density is ED, the laser power is 𝑃, the scan speed is𝑉, and the spot diameter is𝐷 .The sintered process parameters were tabulated in Table 1.
2.3. Characterization. Themorphologies of the scaffoldswere observed with a SEM (JEOL Co., Japan). The technical parameters of SEM were that the resolution was 𝛼 < 3.0 nmandmagnification timeswas 20∼300,000. Before SEM observation, the scaffoldswere platinum coatedwith a sputter coater (JEOL Co., Japan). The scaffolds were analyzed by X- ray diffraction (XRD) (Bruker AXS Inc., Germany) with the Cu target, 𝜆 = 1.54056 Å, and K
𝛼 X-ray. 2𝜃 of XRD graph was
registered in the space (10∘–70∘) at the rate of 2∘/min. Tensile strength of scaffolds was measured by using a
universal mechanical tester (Shanghai Zhuoji Instruments Co. Ltd., China) at environment temperature. The speed of crosshead was selected at 5mm/min and the stress-strain curve was recorded during the tests. Five specimens were tested for each set of process conditions.
2.4. Immersion in SBF. The scaffolds were immersed into simulated body fluid (SBF) to evaluate their in vitro biosta- bility. Ion concentrations in SBF were close to the inor- ganic fraction of blood drug concentration. The SBF solu- tion was obtained by dissolving KH
2 PO 4 , NaHCO
3 , NaCl,
MgSO 4 ⋅7H 2 O,CaCl
2 , andKCl into aqua destillata and buffer-
ing with Tris-HCL to pH 7.4 at human body temperature (37∘C) .The scaffolds were soaked in SBF for 1, 4, 7, and 14 days at human body temperature (37∘C). They, after removal from the fluid, were rinsed with deionized water and dried in cryogenic nitrogen airflow and then weighed. The weight remaining percentage was calculated by
Weight remaining % = 100 − 𝑊
× 100, (2)
where the initial dry weight is 𝑊 0 and the weight after
immersing in SBF is𝑊 𝑡 .
2.5. Cell Culture. To evaluate the biocompatibility of the scaffolds, a cell culture research was carried out. Before the experiment, the scaffolds were sterilized. In detail the process was described as follows: the samples were immersed in 70% ethyl alcohol solution 2 h and afterwards rinsed twice in phosphate buffered saline to shift the ethyl alcohol, followed by exposure to ultraviolet light 15min for each side.
MG63osteoblast-like cells were used for the assessment of the biocompatibility of the scaffolds. The cells were fostered in Dulbecco’s modified Eagle’s medium (DMEM, HyClone, USA) under normal situation. Besides, 10% fetal bovine serum and gentamicin were added into DMEM. Approxi- mately 50 𝜇L of culture medium containing 5 × 104 cells was planted on the scaffolds and cultured for 1, 3, and 5 days in condition of 5%CO
2 at human body temperature (37∘C).The
solution was changed every second day.
2.5.1. SEM Techniques. The cell morphologies on the scaffold were investigated using SEM. After the preselected fostering days, the scaffolds were rinsed with phosphate buffer saline (PBS) two times following settlement with 4% formalin in PBS (pH 7.4). Finally, the scaffolds were rinsed with PBS two times and dewatered in a gradient ethanol series from 50 to 100%.The scaffolds were air drying in a dryer overnight.They were then coated with platinum for SEM observation.
2.5.2. Fluorescence Techniques. Fluorescence technique was used to analyse cell-material interaction. After the cell cul- ture experiment, cells were cleaned with PBS, settled with paraformaldehyde (Sigma, St. Louis, MI, USA), washed, and then permeabilized with 0.1% Tween 20. Afterwards, the cell was rinsed with PBS and then preincubated by 1% gelatin in PBS 20 minute prior to incubation in a compound of 4𝜇M EthD-1 and 2 𝜇M calcein AM in PBS for 30min in a humid chemostat. Fluorescence figures were achieved straightway with a confocal microscope (Leica Microsystem, Mannheim, Germany).
2.6. Statistical Analysis. Theexperimental data were analyzed by origin 8.0 software and the results were depicted as
International Journal of Polymer Science 3
10 20 30 40 50 60 70 0